Effects of Gas Composition on Highly Efficient Surface Modification of Multi-Walled Carbon Nanotubes by Cation Treatment
- First Online:
- Cite this article as:
- Tseng, W., Tseng, C. & Kuo, C. Nanoscale Res Lett (2009) 4: 234. doi:10.1007/s11671-008-9231-4
- 1.8k Views
High incident energy hydrogen and/or oxygen cations are generated by electron cyclotron resonance system, and then used to highly efficiently modify multi-walled carbon nanotubes (MWCNTs). The effects of various H2/O2 gas compositions on the modification process are studied. A systematic characterization method utilizing a combination of X-ray photoelectron spectroscopy (XPS), scanning electron microscopy, Raman spectroscopy, and thermogravimetric analysis (TGA) is used to evaluate the effects of various H2/O2gas compositions on MWCNT functionalization. The Raman results show that the ID/IG ratio is directly affected by H2 concentration in gas mixture, and the treatment applying a H2/O2 gas mixture with ratio of 40/10 (sccm/sccm) can yield the nanotubes with the highest ID/IG ratio (1.27). The XPS results suggest that the gas mixture with ratio of 25/25 (sccm/sccm) is most effective in introducing oxygen-containing functional groups and reducing amorphous carbon. The TGA suggests that the structural change of the treated nanotubes is marginal by this method with any gas condition.
KeywordsMulti-walled carbon nanotubesElectron cyclotron resonance plasmaX-ray photoelectron spectroscopyFunctionalizationRaman spectroscopy
Recently, nanostructured materials have attracted intensive attention in many applications because of their unique properties [1–4]. As one of the most promising materials, and to make the best use of their singular properties, carbon nanotubes (CNTs) can be modified or prepared by different processes to meet the requirements of specifically potential applications [5–7]. The process of facially modifying the nanotubes through changing their surface structure is a relatively simple technique and has been widely investigated [8–10]. The main premise behind these methods is to affix highly polar functional groups to the surface of the nanotubes to enhance their polarity so as to disperse them in the aqueous or polymer matrix. Currently, acid treatment is the most commonly used technique for this process. However, it is mentioned that the use of harsh acids would give rise to issues concerning the drastic changes of the structural integrity, length, and even useful properties of the nanotubes [11–15].
Recently, plasma treatment has been proven to be an attractive alternative and has become increasingly popular in the functionalization of CNTs because the procedure is solvent-free, time-efficient, versatile, and environmental friendly [16–23]. To date, many approaches have been investigated to demonstrate the viability and performance of plasma treatment for surface functionalization of CNTs. In these studies, various gases, such as N2 , H2, O2 [19–21], NH3 [16, 19, 20], and CF4 [19, 23] have been used. Generally, the plasma is generated using glow discharge, radio frequency discharge, or microwave discharge at low-vacuum pressure. The high-energy particles generated in the plasma can then satisfy the chemical bonding energies on the surface of the tubes thereby initiating chemical reactions. In addition, their density and energy can be readily regulated by external parameters, such as the electromagnetic frequency, power, and gas pressure, to achieve optimum conditions for the required production scale and efficiency . However, some studies mention that the nanotubes could be overheated by hyperthermal plasma [19, 21].
In our previous study, through using H2/O2 gas mixture as etching gas, electron cyclotron resonance (ECR) plasma treatment was shown effective to functionalize multi-walled carbon nanotubes (MWCNTs) with minor negative consequences in nanotube structure . In the process, high incident energy hydrogen and oxygen cations generated and extracted by ECR plasma system were used to create free radical defects on the surface of the MWCNTs through ion bombardment; oxygen cations with the high reduction potential present in the ion stream were simultaneously involved in initiating covalent bonding reactions on the surface of the tubes. The ratio of H2 to O2 is critical to the process because it directly correlates with the composition of the generated cations. In this study, the effect of gas composition on the functionalization process is investigated, by providing various H2/O2 gas mixtures to the treatment through the control of gas flow ratio. Furthermore, the manner in which the gas conditions correlate with morphology and structural changes of the nanotubes will be studied through the use of some advanced instruments.
In order to evaluate the surface morphology and structural changes, the samples were dispersed on a silicon wafer using ethanol and measured using scanning electron microscopy (SEM) (JEOL, JSM-6500F). The microstructure of the pristine sample was characterized by transmission electron microscopy (TEM) (JEOL, JEM-2100) through dispersing sample powders on Lacey carbon grids using ethanol. X-ray photoelectron spectroscopy (XPS) was performed to determine the chemical changes at the surface of the nanotubes. Thermogravimetric analysis (TGA) (TA-500) was applied to investigate the changes in thermal stability with a heating rate of 10 °C/min and an air flow of 60 mL/min. Raman spectroscopy (Jobin YVON LabRam HR800) was used to evaluate structural defects in the CNTs.
Results and Discussion
The MWCNT specimen treated under various H2/O2gas compositions; the characterization results of XPS; and theID/IGratio of Raman spectra
As expected, allID/IGratios are increased after plasma treatment with any gas composition. As shown in the inset of Fig. 6, theID/IGratio increases from 1.03 to 1.27 when the H2concentration increases from 0 to 80 vol.%. Note that the ion density is very important for surface etching. By comparing the ionic current, it is found that current increases from 0.12 to 0.47 A while the H2concentration increases from 0 to 100%. This shows that the ion density of the cation stream increases as H2concentration increases. This leads to higherID/IGratio when H2concentration of the etching gas is higher. However, it is also shown that the ratio decreases to 1.08 when the nanotubes are treated with pure H2gas (H2/O2of 50/0 (sccm/sccm)). This could be because the ion bombardment under this gas condition can heavily etch the surface of the nanotubes to the extent that the concentration of amorphous carbon coated on the surface could thus be raised from 40 to 54% as shown in Table 1. The thick amorphous carbon can prevent defects from further forming on the surface during ion bombardment so that theID/IGratio is significantly smaller than that of the nanotubes treated with the etching gas containing 20 vol.% oxygen (ID/IG = 1.27, H2/O2of 40/10 (sccm/sccm)). Apart from their involvement in ion bombardment, the generated oxygen cations can also act as highly reactive chemical species which form covalent bonds with the amorphous carbon and then nanotube surface. More specifically, the amorphous carbon layer is more reactive than the cylindrical walls to form volatile products with the oxygen cations. The products are then pumped out by the vacuum system. Thus, as shown in Table 1, treatment using a H2/O2mixture can increase the concentration of oxygenated functional groups whilst also reducing the concentration of amorphous carbon. On the other hand, treatment with pure O2gas (with the exception of increasing theID/IGratio) does not yield any other obvious effects in regard to the purity of CNTs and the concentration of functional groups when compared with the pristine MWCNTs. This indicates that a H2/O2mixture not only facilitates defect formation but also promotes covalent bonding in this case. Therefore, even with the addition of 20 vol.% H2(H2/O2of 10/40 (sccm/sccm)) in gas, there is still a significant removal of amorphous carbon and formation of oxygen-containing groups on the nanotube surface.
In this article, the effects of various H2/O2gas compositions on the functionalization of MWCNTs using ECR plasma system are studied. The results of Raman spectroscopy show that the cation treatment is effective in introducing defects to the nanotube surface; and this is affected by H2concentration in gas mixture provided. Meanwhile, with a H2/O2mixture of 40/10 (sccm/sccm), the treatment can produce nanotubes with highestID/IGratio (1.27). As demonstrated by the characterization results of XPS, the gas composition strongly correlates with the functionalization extent and amorphous carbon removal. As compared to the other gas composition applied in this study, the treatment using a H2/O2mixture of 25/25 (sccm/sccm) is found to be the most effective gas mixture to graft oxygen-containing functional groups and remove the amorphous carbon on the surface of the nanotubes. Specifically, by using this gas condition to conduct the plasma treatment, the highest concentration of 31.1% (after 5 min exposure) of oxygenated functional groups on the surface of CNTs is achieved. In addition, the amorphous carbon can also be significantly removed. On the other hand, the results also indicate that the structural and morphological changes, if any, are marginally effected by this method with any gas composition.